Enhanced band-edge photoluminescence from ZnO-passivated ZnO nanoflowers by atomic layer deposition
© Ai et al.; licensee Springer. 2013
Received: 7 November 2012
Accepted: 27 January 2013
Published: 25 February 2013
The ZnO nanoflowers were synthesized by reactive vapor deposition. A secondary nucleation in the stalk/leaves interface was suggested. The photoluminescence revealed that there were many oxygen vacancies in the nanoflowers. To tune the optical properties of ZnO nanoflowers, ZnO thin films with varying thicknesses were coated on the nanoflowers by atomic layer deposition, which can distinctly improve the band-edge photoluminescence properties.
KeywordsZnO nanoflowers Atomic layer deposition Photoluminescence 77.55.hf 73.63.Bd 73.40.Kp
Recently, one-dimensional (1-D) zinc oxide nanostructures including nanocages , nanotubes , cylindrical nanowires , nanorods , nanoribbons, and belt-like nanostructures have been obtained. Zinc oxide nanostructures attracted much attention due to their wide direct band gap of 3.37 eV and large exciton binding energy of 60 meV at room temperature [5–12] and their great potential applications in solar cells , piezoelectric devices , gas sensors , and UV laser diodes . ZnO nanostructures can be synthesized by reactive vapor deposition under controlled conditions. By changing the growth conditions, different ZnO nanostructures have been prepared. On the other hand, atomic layer deposition (ALD) is good at control of the accuracy, homogeneity, consistency, and thickness of the thin coatings, which brings it to be a good way for the surface modification and enhancement.
In this work, we demonstrate the growth of ZnO nanoflowers by reactive vapor deposition. To improve the optical properties, the ZnO thin films with varied thicknesses from 15 to 45 nm were coated on the nanoflowers by ALD. This thin-coated layer does not change the morphologies of the sample but can greatly improve its optical properties.
The growth of ZnO nanostructures was performed in a horizontal tube furnace. Zn powder (99.9%) with a weight of 1 g was loaded in quartz boat and placed into the center of the tube furnace, and the clean Si substrates were located at 2 cm downstream from the Zn source. Afterwards, the tube furnace was heated to 440°C with a rate of 20°C/min and held there for 60 min. During the whole synthesis process, a constant flow of O2/Ar mixed gas (5%) at 30 sccm was introduced into the system and the pressure in the tube was kept about 200 Pa.
The as-grown ZnO nanoflowers were coated with thin ZnO layers grown by ALD with a TSF-200 machine (Beneq Oy, Vantaa, Finland). Diethyl zinc (DEZn) and deionized water (H2O) were used as the sources of zinc and oxygen, respectively. High-purity nitrogen carrier gas was used to load DEZn and H2O to the chamber and cleanse the redundant former precursor. The temperature of the substrate was held at 200°C. In each identical ALD cycles, DEZn was introduced into the chamber firstly for 0.2 s, and afterward the chamber was purged by N2 for 1 s. In succession, H2O was introduced into the chamber for 0.2 s followed by another purging procedure at 1 s. The thickness of the ZnO film was about 15 nm after 100 cycles were performed.
X-ray diffraction (XRD; Bruker D8 Advance, Bruker AXS GmbH, Karlsruhe, Germany) and high-resolution transmission electron microscopy (HRTEM, JEOL JEM 2010 FEF UHR; JEOL Ltd., Tokyo, Japan) were used to analyze the crystallization and the microstructure of the ZnO nanoflowers. The morphologies of the sample were characterized by a Sirion (FEI Company, OR, USA) FEG scanning electron microscope (SEM). The photoluminescence (PL, Horiba LabRAM HR800; HORIBA Jobin Yvon S.A.S., Longjumeau, Cedex, France) spectra were utilized at room temperature in a wavelength range of 350 to 700 nm to analyze the optical properties of the ZnO nanoflowers and the coated films.
Results and discussion
The nanowires in the junction of the branch are not very smooth. Therefore, we suggest that this branching should not be the epitaxy of a nanowire crystal face. It belongs to the secondary nucleation phenomena, which means that the nanowires grow to a certain length along the c-axis and a secondary nucleation appears at the top the nanowire. These crystal nuclei grow along the new nuclear c-axis and form a flower-like structure. To verify our hypothesis, the samples were analyzed by transmission electron microscopy (TEM) in the following text.
Figure 2a shows the TEM image of the nanoflower structure of the nanowires. Figure 2b shows the HRTEM image of the region marked by the white square b in Figure 2a, which is located in the stalk. The interplanar distance of 0.26 nm is corresponding to the wurtzite ZnO (0002) planes; hence, the growth orientation is along the c-axis. Figure 2c is the enlarged image corresponding to the region marked by the white square c in Figure 2a. A gap can be observed at the joint parts between the stalk and leaves, which is marked by the white circle in Figure 2c. This suggests that the leaves structure does not belong to the same epitaxial structure of the stalk, but rather due to the secondary nucleation. The growth mechanism of the nanoflower structure can be described as below: First, the nanowire grows along c-axis direction with a wurtzite structure. Then in the top region of the nanowire, there is secondary nucleation, and the c-axis of the new ZnO grains deviates from the direction before. The end planes of the leaves structures show the regular hexagon. These branches exhibit symmetry due to the constraints from space position.
To improve the optical properties, the as-grown sample was coated by a ZnO thin film by ALD. It was shown that ZnO films grown by ALD would have few zinc interstitials and oxygen vacancies ; hence, it is a good way to improve the optical properties of the nanostructures. After a ZnO film was coated, with thickness about 15 nm (the blue squares), the deep-level emission decreased dramatically about 80%; moreover, the intensity of band-edge transition increased about 30%. The ratio α is about 1.65. This result reveals that the very thin film on the surface of the nanoflowers can effectively enhance their optical properties without altering the morphologies.
With the increasing thickness in the coating of ZnO films, the deep-level emission decreases and the band-edge transition increases, as shown in Figure 6. The deep-level emission of the sample coated with 45 nm ZnO is only 4% of that from the as-grown sample. In addition, the intensity of the band-edge transition from the sample coated with 45-nm ZnO is 300% more than that from the as-grown sample. The ratios of the intensity of the band-edge transition to the deep-level emissions are 5.91 and 16.5 for the samples with 30-nm and 45-nm ZnO, respectively.
These results show that an ALD coating of ZnO thin films can effectively enhance the optical properties of the ZnO nanostructures. However, we should know whether the PL result is due to the original ZnO nanoflower or from the ALD ZnO. Hence, we fabricated the ZnO thin film on silicon substrate by ALD using the same parameters. The thickness of this ZnO film is 45 nm, and the PL spectrum of this sample is shown as the inset of Figure 6. A strong peak around 382 nm can be observed, which is attributed to the band-edge transition. Moreover, there is nearly no deep-level emission in the sample. Hence, we can make a conclusion that the stronger peak of the band-edge transition is mostly from the ZnO thin films by ALD, while the weaker peak of the deep-level emission is from the original ZnO nanoflowers. Usually, in the ZnO nanostructures, there are many oxygen vacancies and zinc interstitials, so their optical properties are very poor. Our result reveals that we could coat an epitaxial ZnO thin film by ALD on these nanostructures. This method can effectively enhance the optical properties without changing the morphologies.
Another point should be noted that there is a blue shift in the band-edge transitions and a red shift in the deep-level emissions with increasing the thickness of the coating ZnO films. This reason needs further investigation.
In conclusion, we have synthesized ZnO nanoflowers by reactive vapor deposition. The ZnO thin films were coated on the pristine nanostructures by ALD. These thin-coated layers could remarkably improve the UV band-edge photoluminescence of the nanoflowers without changing their morphologies. Our method can provide an effective way to enhance the performance of the possible ZnO nanostructure devices.
This work is supported by the National Natural Science Foundation of China under grants 10904116, 11074192, 11175135, and J0830310, the foundation from CETC No. 46 Research Institute and the Fundamental Research Funds for the Central Universities 2012202020215, 2012202020210. The authors would like to thank QK Jiang for the technical support.
- Saito Y, Matsumoto T: Carbon nano-cages created as cubes. Nature (London) 1998, 392: 237.View ArticleGoogle Scholar
- Chopra NG, Luyken RJ, Cherrey K, Crespi VH, Cohen ML, Louie SG, Zettl A: Boron nitride nanotubes. Science 1995, 269: 966. 10.1126/science.269.5226.966View ArticleGoogle Scholar
- Morales AM, Lieber CM: A laser ablation method for the synthesis of crystalline semiconductor nanowires. Science 1998, 279: 208. 10.1126/science.279.5348.208View ArticleGoogle Scholar
- Dai HJ, Wong EW, Lu YZ, Fan SS, Lieber CM: Synthesis and characterization of carbide nanorods. Nature (London) 1995, 375: 769. 10.1038/375769a0View ArticleGoogle Scholar
- Huang MH, Mao S, Feick H, Yan H, Wu Y, Kind H, Weber E, Russo R, Yang P: Room-temperature ultraviolet nanowire nanolasers. Science 1897, 2001: 292.Google Scholar
- Kong YC, Yu DP, Zhang B, Fang W, Feng SQ: Ultraviolet-emitting ZnO nanowires synthesized by a physical vapor deposition approach. Appl Phys Lett 2001, 78: 407. 10.1063/1.1342050View ArticleGoogle Scholar
- Yang P, Yan H, Mao S, Russo R, Johnson J, Saykally R, Morris N, Pham J, He R, Choi HJ: Controlled growth of ZnO nanowires and their optical properties. Adv Funct Mater 2002, 12: 323. 10.1002/1616-3028(20020517)12:5<323::AID-ADFM323>3.0.CO;2-GView ArticleGoogle Scholar
- Wang X, Summers CJ, Wang ZL: Large-scale hexagonal-patterned growth of aligned ZnO nanorods for nano-optoelectronics and nanosensor arrays. Nano Lett 2004, 4: 423. 10.1021/nl035102cView ArticleGoogle Scholar
- Bai XD, Gao PX, Wang ZL, Wang EG: Dual-mode mechanical resonance of individual ZnO nanobelts. Appl Phys Lett 2003, 82: 4806. 10.1063/1.1587878View ArticleGoogle Scholar
- Lao JY, Huang JY, Wang DZ, Ren ZF: ZnO nanobridges and nanonails. Nano Lett 2003, 3: 235. 10.1021/nl025884uView ArticleGoogle Scholar
- Gao PX, Lao CS, Yong D, Wang ZL: Metal/semiconductor core/shell nanodisks and nanotubes. Adv Funct Mater 2006, 16: 53. 10.1002/adfm.200500301View ArticleGoogle Scholar
- Kong XY, Yong D, Yang R, Wang ZL: Single-crystal nanorings formed by epitaxial self-coiling of polar nanobelts. Science 2004, 303: 1348. 10.1126/science.1092356View ArticleGoogle Scholar
- Law M, Greene LE, Johnson JC, Saykally R, Yang P: Nanowire dye-sensitized solar cells. Nat Mater 2005, 4: 455. 10.1038/nmat1387View ArticleGoogle Scholar
- Kong XY, Wang ZL: Spontaneous polarization-induced nanohelixes, nanosprings, and nanorings of piezoelectric nanobelts. Nano Lett 2003, 3: 1625. 10.1021/nl034463pView ArticleGoogle Scholar
- Wan Q, Li QH, Chen YJ, Wang TH, He XL, Li JP, Lin CL: Fabrication and ethanol sensing characteristics of ZnO nanowire gas sensors. Appl Phys Lett 2004, 84: 3654. 10.1063/1.1738932View ArticleGoogle Scholar
- Lee ST, Liu CH, Zapien JA, Yao Y, Meng XM, Lee CS, Lifshitz Y, Fan SS: High-density, ordered ultraviolet light-emitting ZnO nanowire arrays. Adv Mater 2003, 15: 838. 10.1002/adma.200304430View ArticleGoogle Scholar
- Wang T, Wu H, Chen C, Liu C: Growth, optical, and electrical properties of nonpolar m-plane ZnO on p-Si substrates with Al2O3 buffer layers. Appl Phys Lett 2012, 100: 011901. 10.1063/1.3673346View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.